Surface Conditioning of NiTi and Ta NiTi sheets and NiTi stents:The device used for elec-trochemical
Embed Size (px)
Transcript of Surface Conditioning of NiTi and Ta NiTi sheets and NiTi stents:The device used for elec-trochemical
September 2001 439
Metallic coronary stents are medical devices that pro- vide endovascular scaffolding to relieve vascular obstruction. They exert a continuous radial pressure on the diseased coronary artery, resulting in a compres- sion of atherosclerotic plaques, sealing of dissections, and expansion of the coronary vessel [1,2]. When used as an adjunct to conventional balloon angioplasty, they improve vessel patency [3,4]. Surface roughness is an important determinant of thrombogenicity and tissue reaction ; the nature of the metal surface is crucial to blood compatibility . A smooth surface can help to prevent the activation and aggregation of platelets, which is recognized to be one component of the process of thrombosis. A previ- ous experimental investigation with animals  has shown that surface treatment can modify the perfor- mance of stents. In the animal experiments, the results of implantation of both polished stainless steel and nitinol stents were compared with those of unpolished stents. The conclusions are that metallic surface treat- ment with polishing effectively results in decreased thrombogenicity [5,7].
The most important clinical problem after stent implantation remains neointimal hyperplasia within the stent, resulting in significant stent narrowing in 16 – 30 % of patients [2,3,8-10]. Further efforts to improve the clinical results of coronary stents should focus on decreasing this neointimal hyperplasia. Not only have previous studies with animal models shown that metallic surface treatment using electrochemical polishing decreased the thrombogenicity, but they also showed a decrease in the neointimal hyperplasia of coronary stents [11,12]. Some studies have shown that a smooth surface on the stents could improve the efficiency of healing. Thus, polishing various metallic stents has shown its impor- tance in the material aspects of the study of the stents. Electrochemical polishing is a process in which a metallic surface is smoothed by polarizing the anode in an appropriate electrolytic solution . Electro- chemical polishing is classified into two processes: anodic leveling and anodic brightening . Anodic leveling results from a difference in the dissolution rate between peaks and valleys on a rough metal surface
Progress in Biomedical Research
Surface Conditioning of NiTi and Ta Stents
H. ZHAO, J. VAN HUMBEECK Department of Metallurgy and Materials Engineering, Katholieke Universiteit Leuven, Heverlee, Belgium
I. DE SCHEERDER Department of Cardiology, University Hospital Gasthuisberg, Katholieke Universiteit Leuven, Leuven, Belgium
The present study explores the optimal methods for polishing NiTi and Ta stents. Electrochemical polishing was explored and several parameters were investigated including applied voltage, polishing time, and acid pickling prior to the polishing process. As a comparison, chemical polishing was also conducted. Both mechanical and elec- trochemical polishing of NiTi sheet materials were investigated to study the influence of electrochemical polishing on the surface composition of NiTi stents. Pickling was necessary prior to electrochemical polishing in order to remove the oxide films covering the stent surface. The surface quality of the NiTi and Ta stents significantly improved when the optimal condition for polishing was achieved.
Stents, electrochemical polishing, mechanical polishing, acid pickling
440 September 2001
Materials and Methods
Materials The original materials used in this study were a cold- rolled binary near-equiatomic NiTi rolled sheet (length 100 mm, width 5 mm, and thickness 1.4 mm, AMT, Belgium), binary near-equiatomic NiTi wires with diameters of 1 mm (Krupp, Germany), 0.5 mm, and 0.3 mm (both from AMT, Belgium), non-polished NiTi stents (φ 2.5 × 20 mm, φ 2.5 × 15 mm, and φ 2.5 × 10 mm, research products from Global Therapeutics, USA) and non-polished tantalum stents (φ 2.0 × 15 mm, research products from Medtronic, USA). The NiTi sheet was used to study the differences between mechanical and electrochemical polishing. The NiTi wires were used to explore the different conditions for electrochemical polishing of NiTi coil stents. The sam- ples were cleaned for 10 min in an ultrasonic agitation bath using an alkaline solvent with a detergent additive (RW77, Tickopur, Bandelin, Germany). Then they were cleaned for > 10 min using distilled water in an ultrasonic agitation bath and were air-dried.
Acid Pickling Acid pickling is an effective method for the chemical removal of surface oxides and other contaminants from metallic materials by immersion in an aqueous acid solution . NiTi sheets and NiTi stents: The sheets were immersed in the acid solution  (Table 1) for 1, 4, 7, 10, and 14 min at room temperature. Due to the oxides formed
depending on the current distribution or mass-transport conditions. Anodic brightening is associated with the suppression of the influence of the metal microstructure on the dissolution rate. A smooth electrochemically polished surface, which appears bright to the naked eye, results from a combination of these two factors . Previous studies on the surface conditioning of stainless steel stents have shown the effects of electrochemical polishing on the efficiency of physiologic healing. Other studies focused on the electrochemical polishing of other types of stents. The aim of this paper is to investigate and determine the optimal conditions for electrochemically polishing nickel-titanium "nitinol" (NiTi) and tantalum (Ta) stents.
Progress in Biomedical Research
Table 1. Composition of pickling solution for NiTi sheets and NiTi stents.
Table 2. Composition of pickling solution for Ta stents.
Table 3. Electrolytes (a) for polishing NiTi sheets and NiTi stents and conditions for polishing of NiTi sheets (b).
September 2001 441
during the manufacturing process, the stents were also immersed in the acid solution for another 1, 2, 4, 6, and 8 min at room temperature. Ta stents: After being degreased the Ta stents were immersed in an acid solution (Table 2) for 2.5, 5, 7.5, 10, and 20 min at room temperature; this was done to remove the oxides on the stent struts. After being pick- led, all the samples were rinsed with distilled water in an ultrasonic agitation bath for > 10 min and were then air-dried. Evaluation of the results was done by obser- vation with a stereomicroscope (Wild Heerburg, Switzerland).
Chemical Polishing NiTi sheets and NiTi stents: Chemical polishing was done to compare the polishing effect with electro- chemical polishing using the acid solutions H2O2 and HF, i.e. electrolytes (iii) and (iv) listed in Table 3a. After being pickled for 7 min, the NiTi sheets were immersed in the selected acid solutions for 3, 9, and 15 min at room temperature (Table 3b). Ta stents: Chemical polishing of the Ta stents was per- formed in an acid mixture (H2SO4, HNO3, and HF), i.e., electrolyte (iii) listed in Table 3a. After pickling the stents were immersed in the selected acid solution for 2, 4, and 6 min at room temperature. After chemi- cal polishing, all the samples were rinsed in distilled water in an ultrasonic agitation bath for > 10 min and then air-dried.
Electrochemical Polishing NiTi sheets and NiTi stents: The device used for elec- trochemical polishing of NiTi sheets and NiTi stents was self-designed. A 150-ml glass beaker was used as a cell. A DC rectifier (Polipower, Struers, Denmark) was used as the power supply, and the cathode was a stainless steel 316L sheet material (length 15 cm, width 2.5 cm, and thickness 0.2 cm). Electrochemical polishing of NiTi sheets was performed with the selected electrolyte  (perchloric acid 70 % and acetic acid 99.8 %) presented in Table 3a. Prior to electrochemical polishing, a pre-treatment using acid pickling was done for 7 min. Several parameters were evaluated to obtain the optimal polishing conditions (Table 3b). They included the electrolyte, the applied voltage, and the polishing time. Initially, the applied voltages (5, 10, 15, 20, and 25 V) were tested with a fixed time of 10 min using electrolyte (i). Then the applied voltages were fixed to 20 and 25 V respective-
Progress in Biomedical Research
Table 4. Conditions for electrochemical polishing of NiTi wires (a), NiTi stents (b), and NiTi stents (c) without pick- ling.
Table 5. Electrolytes (a) and conditions (b) for polishing of Ta stents.
442 September 2001
Electrochemical polishing of NiTi wires was per- formed with different parameters including the applied voltages and the polishing times to find an optimal set- ting for electrochemical polishing of NiTi stents. The wires were ground with rough abrasive paper prior to electrochemical polishing. The conditions for electro- chemical polishing of NiTi wires are summarized in Table 4a. Selection of these conditions depended on the results of electrochemical polishing of the sheet materials. Several applied voltages (20, 25, and 30 V) were tested for different times (2, 3, 4, and 8 min) using electrolyte (ii) at room temperature without stir- ring. Based on the experiences of electrochemically polish- ing both NiTi sheets and NiTi wires, electrochemical polishing of NiTi stents was conducted. After a 6 min pre-treatment with acid pickling followed by a rinse, electrochemical polishing of NiTi stents was evalu- ated with different parameters including the applied voltages and the polishing times. The conditions for electrochemical polishing stents are summarized in Table 4b. These conditions were s